{'fraction_non_alphanumeric': 0.033664599790481045, 'fraction_numerical': 0.025935049123701124, 'mean_word_length': 4.91723906852069, 'pattern_counts': {'":': 0, '<': 2, '<?xml version=': 0, '>': 1, 'https://': 0, 'lorem ipsum': 0, 'www.': 8, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 1, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Polysaccharide hydrogel based 3D printed tumor models for chemotherapeutic drug screening

A series of stable and ready-to-use bioinks have been developed based on the xeno-free and tunable hydrogel (VitroGel) system. Cell laden scaffold fabrication with optimized polysaccharide-based inks demonstrated that Ink H4 and RGD modified Ink H4-RGD had excellent rheological properties. Both bioinks were printable with 25–40 kPa extrusion pressure, showed 90% cell viability, shear-thinning and rapid shear recovery properties making them feasible for extrusion bioprinting without UV curing or temperature adjustment. Ink H4-RGD showed printability between 20 and 37 °C and the scaffolds remained stable for 15 days at temperature of 37 °C. 3D printed non-small-cell lung cancer (NSCLC) patient derived xenograft cells (PDCs) showed rapid spheroid growth of size around 500 µm in diameter and tumor microenvironment formation within 7 days. IC50 values demonstrated higher resistance of 3D spheroids to docetaxel (DTX), doxorubicin (DOX) and erlotinib compared to 2D monolayers of NSCLC-PDX, wild type triple negative breast cancer (MDA-MB-231 WT) and lung adenocarcinoma (HCC-827) cells. Results of flow property, shape fidelity, scaffold stability and biocompatibility of H4-RGD suggest that this hydrogel could be considered for 3D cell bioprinting and also for in-vitro tumor microenvironment development for high throughput screening of various anti-cancer drugs.

components [16][17][18] . VitroGel is a ready-to-use, xeno-free hydrogel system for 3D cell culture research. It can be modified with multi-functional ligands and mechanical strength to closely mimic the natural extracellular matrix (ECM) environment to support a wide range of cell types for different applications. The hydrogel is room temperature stable, has a neutral pH, transparent, permeable and compatible with different imaging systems. The solution transforms into a hydrogel matrix by simply mixing with the cell culture medium.
Biocompatibility, hydrophilicity, biomimetic ability, bio-processability, biodegradability, and affordability of the bioinks are also taken into consideration during 3D printing of cell laden scaffolds 16 . During 3D printing, less viscous bioinks easily flow through the narrow printing nozzle but they have the drawbacks of smearing and low shape fidelity 12,19 . Highly viscous bioinks can give better shape resolution by using high extrusion pressure 16,19 but creation of high shear force in the printing nozzle by application of higher extrusion pressure causes cell destruction during printing process 16,20 . So, optimizing the flow properties is the primary criteria of printable bioinks [21][22][23] .
Polymer crosslinking method is also another key parameter of the bioink for 3D printed scaffolds fabrication [24][25][26] . Crosslinking by hydrogen bonds, crystallization, ionic interactions and protein interaction are examples of physical crosslinking mechanisms 26,27 . Physically crosslinked bioinks are usually associated with poor mechanical stability. Covalent bonding between polymer and crosslinker functional groups is an example of chemical crosslinking mechanisms 28 . Among various methods, covalent crosslinking is proved to be an effective method for improving the physiological stability of printed structures 29,30 . However, toxicity and unwanted reactions of the crosslinker with the bioactive substances present in the hydrogel matrix limit their application. Changes in pH and temperature, high energy radiation, free radical polymerizations can be used for crosslinking in 3D cultures 27 .
In this study, we hypothesize to test a series of room temperature stable and ready-to-use hydrogels by working in collaboration with TheWell Bioscience (North Brunswick, NJ 08902) company. Our goal is to develop a hydrogel which mimics the in-vivo tumor microenvironment, shows good printability, rheological characteristics (i.e., shear-thinning and rapid recovery rheological properties of hydrogels can lead to a stable printed structure after extrusion), biocompatibility and also can be used for application of screening of anti-cancer drugs. As current crosslinking methods of bioinks such as sudden changes in temperature, chemical reactions, and exposure to high energy radiation (UV light) could cause destruction to the cells during the process of solidification of printed scaffold after hydrogel extrusion 31,32 , we would also like to have our printed cell laden scaffolds developed with characterized hydrogel have additional property of getting crosslinked with the cell culture media, maintaining good biocompatibility and stability for long periods of time. Since there are no requirements of crosslinking through temperature changes, chemicals and radiation during bioprinting, this novel bioink could be an easy-to-use system to carry out comparative cytotoxicity testing of various anticancer drugs in 3D printed spheroids and conventional 2D cultures.

Results
Bioink optimization for scaffold fabrication and bioink cytocompatibility studies. After testing a series of room temperature stable and ready-to-use hydrogels received from TheWell Bioscience (North Brunswick, NJ 08902), we found that Ink H4 and its modified form, H4-RGD showed high shape fidelity along with high cell viability. Both the hydrogels showed good viability of MDA-MB-231 WT cells after immediate postprinting evaluation by performing Calcein AM/Ethidium homodimer III staining, which showed the images of live (stained green) and dead (stained red) cells (Fig. 1A) and the percentage of cell viability (Fig. 1B) was calculated by NIH ImageJ software. We observed that both these inks were printed under pressure conditions ranging from 25 to 50 kPa (Fig. 1C). We observed poor printability with Ink H1 ( Figure 2A shows the photographic image of 10-layer printed scaffold with Ink H4-RGD. The printed scaffolds of Ink H4-RGD displayed designed pore size and good line width without any smearing problems (Fig. 2B,C). Figure 2D shows the fluorescent image of NSCLC-PDX cell laden Ink H4-RGD scaffold stained with calcein. The average Pr (printability) value of 12 Ink H4-RGD scaffolds was 0.96, which indicates that this ink could be considered for 3D printing of cell laden scaffolds. We also investigated the biocompatibility of Ink H4-RGD in various cancer cells and found that all evaluated cell lines of lung cancer (NSCLC-PDX, H460, HCC-827and A549) and breast cancer (MDA-MB-231WT), and bladder cancer (RT4) cells have showed more than 90% cell viability after post printing evaluation as analysed by counting the cell viability through NIH ImageJ software (Fig. 3).
Rheological properties of optimized bioprintable inks. We evaluated rheological parameters to assess and determine the feasibility of inks H4 and H4-RGD for extrusion based bioprinting without additional curing process. Rheological assessments revealed that Ink H4 and Ink H4-RGD displayed shear thinning properties i.e., we observed decrease in the viscosity when the shear rate was increased (Fig. 4A,B) at 25 °C. This suggests that inks H4 and H4-RGD can be used for extrusion based bioprinting. Further, oscillation temperature sweep test demonstrated that Ink H4-RGD displayed stable elastic modulus across wide temperature ranges i.e., at room temperature and physiological temperature (Fig. 4C). Further, we observed that Inks H4 and H4-RGD showed shear thinning and shear recovery properties at both 25 °C and 37 °C (Fig. 5A,B) www.nature.com/scientificreports/ the rheological properties after crosslinking of Ink H4 and H4-RGD with cell culture media in 5:1 ratio. It was observed that crosslinked inks H4 and H4-RGD also showed shear thinning and shear recovery properties at both 25 °C and 37 °C (Fig. 5C,D). However, the recovery rate was faster at 37 °C in comparison to 25 °C, and also faster with 5:1 mixed (partially crosslinked) samples when compared to unmixed samples ( Fig. 5A-D). We observed that all the four samples recovered more than 60% of the elastic modulus instantly after 500% shear strain force was ceased, and almost 100% of the elastic modulus during the 10 min time sweep test, indicating the shear recovery properties of the hydrogel. After the phase 3 test, phase 4 amplitude sweep test was applied to the same samples and we assessed rheological properties. We again observed similar shear-thinning properties of the hydrogel system, further confirming the above results. Since the mechanical strength of the inks can be rapidly recovered after the shearing force was ceased, these inks can maintain the printing structure without further curing process. Inks H4 and H4-RGD have showed pseudoplastic or shear thinning behaviour. The plot of log shear stress vs log shear rate has also showed non-zero intercept. Based on the power law mode equation, we have summarized the flow index (n), flow consistency index (k) and the R 2 values of Ink H4 and H4-RGD at 25 °C, 37 °C and 40 °C in Table 1. The n value was found to be less than 1, which also indicates non-Newtonian pseudoplastic flow properties of Inks H4 and H4-RGD.
Mechanical properties of printable hydrogel and stiffness of cell-laden scaffolds. Based on our printability, cell viability and rheological parameters experimental results, Ink H4-RGD was optimized for 3D printing of cancer cells in-vitro. It was hypothesized that this hydrogel would offer high printability and compressive modulus. Both non crosslinked H4 RGD and partially crosslinked H4-RGD (5:1 of hydrogel and cell culture media) displayed elastic modulus of around 30 kPa after 24 h incubation with excess cell culture medium at 37 °C (Fig. 6A). Further, the stiffness of printed NSCLC-PDX cell laden scaffolds was also evaluated by using oscillation-time sweep measurements on day 1, 5, 10 and 15 (Fig. 6B). The rheological data of cell laden scaffolds showed around 50 kPa elastic modulus and 7 kPa loss modulus during 15 days of incubation. The loss factor was calculated by dividing the average loss modulus with elastic modulus (G″/G′). The loss factor of printed cell laden scaffolds was found to be in between 0.14 and 0.4 during 15 days of incubation period (Fig. 6B).  www.nature.com/scientificreports/ the diameter of spheroids was found to be in the range of 100-500 µm during the first 7 days (Fig. 7A). We also characterised 3D spheroids by using SEM, which showed the presence of spheroids inside the printed scaffold of Ink H4-RGD (Fig. 7B). We checked the growth of 3D NSCLC-PDX spheroids by performing NucBlue/Actin green staining for a period of 7 days (Fig. 7C). Figure 8A depicts the image of 3D NSCLC-PDX spheroids with Ink H4-RGD on day 7 after assessed by using NucBlue/Actin green staining. Further, we assessed the presence of tumor microenvironment by performing immunofluorescence assay for E-cadherin and vimentin, which revealed the expression of cell adhesion molecule, E-cadherin and Vimentin in the printed NSCLC-PDX 3D spheroids (Fig. 8B,C).

Characterization of 3D spheroids and assessment of in-vitro
Comparative 3D and 2D culture platform anticancer drug sensitivity evaluation. We investigated the anti-cancer efficacy of DTX, erlotinib and DOX in the printed 3D cell laden scaffolds formed by using Ink H4-RGD hydrogel and compared their efficacy in 2D monolayers. In all the three tested cell lines (MDA-MB-231WT, NSCLC-PDX and HCC-827), 3D spheroids showed more resistance to DTX, erlotinib and   Table 2). The IC 50 values of DOX in 2D monolayer cells of MDA-MB 231WT and HCC827 were found to be 1.58 and 10.73 µM respectively ( Table 2). The IC 50 values of DOX in 3D printed spheroids of MDA-MB-231WT and HCC-827 cells were found to be 77.35 and 85.35 µM, respectively. The IC 50 values in 3D printed cell spheroids ranged from 3 to 90 folds higher than the 2D counterparts with equivalent cell numbers, all these suggesting that tumor complexity contribute to decreased sensitivity of DTX, erlotinib and DOX in 3D spheroids.

Discussion
Bioprinting techniques are gaining substantial interest in the field of tissue engineering due to their ability to create complex structures. 3D printing of cell laden scaffolds facilitates homogenous cell/spheroids distribution, homogenous drug diffusion through the entire scaffolds and also opens up new avenues for the fabrication of microtissues 33 . Bioprinting of cells with a designed structure closely mimic in-vivo tissue microenvironment during scaffold-based tissue development 34 . Layer by layer printed scaffolds showed higher cell proliferation and growth when compared to conventional non-printed 3D scaffold cultures 35 . Facilitated media diffusion, easy waste removal and relatively homogenous drug diffusion can be achieved by using 3D bioprinting of cell laden scaffolds with designed pore size and good rheological properties when compared to non-printed 3D cultures [36][37][38][39] . Bioprinting can also prevent core necrosis which is the common problem of non-printed polymer-based 3D models 40 . 3D printing has been recently used to develop in-vitro cancer models for chemotherapeutic drug screening 41 . Because of their similarity with the initial avascular growth stage of malignancies, micro-metastases and intra-capillary tumor microregions, 3D spheres of tumor tissue have also been recently explored to investigate and demonstrate the efficacy of various chemotherapeutics 42 . The imperative step in 3D bioprinting is the formulation of a bioink, which mimics tissue specific intercellular microenvironment 43,44 . In this study, a new formulation of VitroGel RGD-PLUS hydrogel system was used for the first time as a printable bioink for tumor tissue fabrication and in-vitro screening of anticancer drugs. It is an animal origin-free polysaccharide hydrogel system, which is modified with RGD peptide for better cell adhesion.   www.nature.com/scientificreports/ As polysaccharide based bioinks do not have cell attachment motif, they are modified with a tripeptide, Arg-Gly-Asp (RGD) to improve the adhesion properties [45][46][47] . During screening of printable bioinks, biocompatibility with cells and medium should be determined before the selection of an ideal bioink [48][49][50] . This is the first study reporting the use of a carbohydrate based bioink, H4RGD for 3D printing of tumor cells and for screening them against anticancer drugs. Mechanism behind the cross-linking involves the interaction of hydrogel molecules with Ca 2+ or Na + from the cell culture medium. This process is slow and forms a soft hydrogel initially. Adding additional cell culture media on top of the hydrogel would allow more ionic molecules to penetrate into the hydrogel matrix, which further saturates the hydrogel cross linking and forms a solid hydrogel. Bioink extrudability, printed structure line width and scaffold pore size are the determining factors for bioinks evaluation in extrusion-based printings 51,52 . Moreover, bioinks having shear thinning properties can easily pass through the micro-sized nozzle and avoid cell destructive shear forces at the printing nozzle 26,[53][54][55] . Highly viscous bioinks could give better shape resolution but they induce clogging problems at the nozzle tip and can decrease the viability of cells due to the application of high extrusion pressure 18,19,26,53,[56][57][58][59] . Low viscous bioinks induce smearing and shape demolition problems 26 . In our study, both Ink H4 and Ink H4-RGD have showed shear thinning and shear recovery properties at ambient temperatures between 25 and 37 °C. Moreover, the recovery-time point of both hydrogels to their original elastic modulus (G′) was observed to be less than one minute after shearing. The shear thinning properties of these inks helped us to print cells with minimum printing pressure, which could also be beneficial for maintaining cell viability. Since the mechanical strength of the ink can be rapidly recovered after the shearing force was ceased, these inks can maintain the printing structure without further curing process. On the other hand, minimum shear duration or rapid recovery properties of the www.nature.com/scientificreports/ hydrogel are helpful for optimum shape fidelity during scaffold construction 60,61 . During printing process, a solid physical appearance of hydrogel has to be broken or disrupted by minimum shear stress or printing pressure so as to facilitate easy bioink flow through a narrow nozzle without any jamming problem and also to decrease printing related cellular stress 19,60 . Due to its rapid shear recovering property, our vitroGel hydrogel system can maintain the printing structure without any smearing problems through immediate curing process. However, optimal stiffness and stability of printed cell laden scaffolds, depend upon the cross-linking methods and elasticity nature of the bioinks 36,62 . Crosslinker concentration and crosslinking time determine the viscosity of the hydrogel system 63,64 . Bioinks of 3D scaffold constructs should have a superior crosslinking method which can maintain good tensile strength of the hydrogels and viability of the cells 65 . Among various methods, covalent crosslinking is proved to be an effective method for improving the physiological stability of printed structures 29,30 . Addition of cell suspension into the bioinks often decreases the viscosity and complicates the evaluation of printability 51 . Kajsa et.al demonstrated  www.nature.com/scientificreports/ the usage of nanocellulose-alginate bioink and 90 mM CaCl 2 (crosslinker) for cartilage tissue engineering 66 . In our study, usage of Ink H4-RGD bioinks demonstrates an advantage of crosslinking with cell culture medium. Due to this crosslinking method, the printed cell laden scaffolds were maintained in good tensile strength throughout the incubation period. In our study, all the rheological data was recorded with relevant parameters such as shear rate, shear stress, shear strain torque, normal forces, and angular frequencies. The viscosity and visco-elasticity of bioinks were evaluated before printing. Further, stiffness and structural integrity of cell laden scaffolds were also determined. Ink H4-RGD displayed less degradability and excellent tensile strength for an extended period of time among all the tested bioinks, suggesting it as a suitable bioink. Inks H4 and H4-RGD showed favourable flow properties when extruded at the printing pressure ranging from 25 to 50 kPa. The loss factor (tan δ) of Ink H4 and H4-RGD showed suitable viscoelasticity for scaffold fabrication. Our results are supported by an earlier study carried out by Katja et al., which showed that bioinks with viscosity range of 30 mPa-6 × 10 7 mPa are printable by extrusion type printer 26 .
Stiffness of the printed cell laden scaffolds plays a crucial role in structural integrity, cell proliferation and tumor spheroid growth 67 70 . In our study, the stiffness (i.e., 30-55 kPa) of cell laden scaffolds demonstrate higher spheroidal growth and proliferation. Moreover, the stiffness of the scaffolds did not alter/change throughout the incubation period. Printed scaffolds resolution also depends on printing speed, temperature and nozzle diameter 58,71 . Printing with smaller nozzle diameters gives high shape resolution, but it requires high extrusion pressure, which can cause cellular damage 71 . In our study, ink H4-RGD was printed with different nozzle diameters ranging from 200 to 410 µm and higher cell viability was observed at a diameter of 410 µm.
Lattice design plays an important role in 3D printing of cell laden scaffold constructs, as it helps in mimicking cellular microenvironment 48,[72][73][74][75] . In 3D printed cell culture models, interconnected porous structure helps for the diffusion of nutrients and waste products 75 . In layer by layer printing, scaffold size and the pore size are the determining factors for their stability 76 . Yong et al. demonstrated that diffusion is superior in 3D grid pattern when compared to non-porous edges 77 . In our study, the designed scaffolds had three layered grid structure with 10 × 10 × 1 dimension, average line width (400 µm) and average inter-scaffold porosity (16 × 10 4 µm 2 ) respectively. This design was favourable for high proliferation of the cells and better nutrients diffusion, which was evident from rapid spheroid formation within seven days of incubation.
3D spheroid cultures can mimic the oxygen and nutrient gradients of in-vivo tumors 78 . Previous anticancer drug studies revealed that 3D spheroids show more chemoresistance in comparison to 2D cell monolayers [79][80][81] . Tumor heterogeneity is responsible for superior drug resistance in 3D spheroids when compared to 2D culture models, which are devoid of essential tumor microenvironment 82,83 . Poor penetration of drugs through the scaffolds and spheroidal microenvironment barriers are also responsible for superior drug resistance in 3D spheroids [84][85][86] . Thus, there is a need to develop drugs with better penetrating ability to the most interior sections of tumors. The 3D matrix of hydrogel-based scaffolds closely mimic the physical barriers of ECM present around in-vivo tumors. Decreased diffusion of anti-cancer drugs through the spheroids and hypoxia could also contribute to drug resistance in 3D cultures 87 . Karlsson et al. demonstrated that 3D spheroids were more resistant than 2D monolayer colon cancer (HCT-116) cells to anticancer drugs 88 . Paclitaxel, an anti-proliferative drug, which normally acts on dividing cells showed drug resistance in 3D spheroids due to its reduced effect in the interior spheroidal region, which consists of quiescent cells 89 . Besides, the dynamic intercellular and cell-ECM interactions have a major role in drug resistance in 3D spheroids 3 .
In our study, we have seeded equivalent number of cells i.e., 5 × 10 4 cells/scaffold/well and evaluated cytotoxicity with DTX, DOX and erlotinib in 2D and 3D bioprinted cultures of NSCLC-PDX, MDA MB 231 WT and HCC-827 cells. IC50 values were significantly higher in 3D spheroids treated with DTX, erlotinib and DOX when compared to 2D monolayers of NSCLC-PDX, MDA-MB-231WT and HCC-B27 cells. These results support that 3D spheroids show more chemoresistance than conventional 2D platforms to DTX, erlotinib and DOX due to the tumor heterogeneity of 3D spheroids. Our results corroborate with previous reports which show that 3D cultures of alginate based scaffolds are highly resistant to DTX when compared to 2D monolayers of both A549 and H460 cells i.e., IC 50 94 . However, we observed that 3D spheroids formed by ink H4-RGD for MDA-MB-231 WT, NSCLC-PDX and HCC-827 cells showed more resistance in comparison to 2D cell monolayers. This possibly suggests the role of tumor microenvironment created by Ink H4-RGD in determining the variability of chemotherapeutics response in 3D spheroids. Decreased diffusion of anti-cancer drugs through the spheroids and hypoxia could also contribute to drug resistance in 3D cultures 87 . Molecular studies are currently in progress to delineate the possible mechanisms for increased chemotherapeutics resistance in 3D cultures when compared to 2D cell monolayers.

Conclusions
Based on the printability, shape fidelity, rheological parameters, scaffolds morphology, cell viability and rapid spheroid formation, Ink H4-RGD was found to be beneficial in developing tumor scaffolds with in-vivo stromal characteristics. This bioink can be crosslinked with cell culture medium, which facilitates good cell growth and scaffold stability. Ink H4-RGD printed NSCLC PDX cell laden scaffolds showed spheroid formation within 7 days. 3D printed spheroids showed more resistance to DOX, DTX and erlotinib in comparison to 2D monolayers of NSCLC PDX, MDA-MB-231 WT and HCC-827 cells. To the best of our knowledge according to the information disclosed by The Well Bioscience (North Brunswick, NJ 08902) company, we only know that these inks simulate the natural extracellular matrix (ECM) environment by providing in-vitro anchorage and homing sites for in-vitro cells and spheroids. This polysaccharide-based hydrogel system (VitroGel) has also shielding and nurturing property, which closely mimics the in-vivo ECM. In comparison to the reported bioinks, Inks H4 and H4-RGD can be printed through extrusion due to their special shear-thinning and rapid recovery rheological properties of the hydrogel system and also can maintain the printed structure without further UV crosslinking. Moreover, these Inks H4 and H4-RGD can be mixed with different growth factors or compounds if needed to support different cell culture applications. DMEM/F12 media was purchased from Genesee Scientific (SanDiego, CA, USA). RPMI media, bFGF and EGF were purchased from Sigma-Aldrich (St. Louis, MO, USA). B27 supplement, NucBlue, Actin-Green reagents were purchased from Life technologies (USA). Live-Dead cell assay reagent was purchased from Biotium Inc (USA). E-cadherin and vimentin antibodies was purchased from Cell Signaling Technology (USA). Antirabbit, anti-mouse FITC and Rh conjugated secondary antibodies were purchased from Santa Cruz Biotechnology (USA). BIO-X and INKREDIBLE 3D bioprinter (CELLINK Inc, Sweden) were used to print all inks.

Methods
Bioink optimization for scaffold fabrication. Ink H4 and H4-RGD were used for printability evaluation. Both these inks were prepared by our collaborator (The Well Bioscience Company). Based on the preliminary studies of VitroGel hydrogel systems, we observed that these formulated bioinks were found to be crosslinkable with cell culture medium. The experiment was designed to test printability of Ink H4 and H4-RGD, to determine crosslinker ratio (hydrogel:cell culture medium), crosslinking time, and also to evaluate printed scaffolds. For crosslinking and gelation study, each sample was diluted with a cell culture medium in the ratio (hydrogel to cell culture medium respectively) of 1:1, 1:2, 1:3, 1:4, 1:5, 2:1, 3:1, 4:1, 5:1, 6:1 and 10:1. For printability test, hydrogels were loaded into 3 mL printing cartridges and then connected to a controllable pressure regulator (0-1000 k pa) on a Bio-X printer. Three-layered (10 × 10 × 1 mm) scaffolds were printed on a petri-dish using 22G nozzle (410 µm diameter) and the printability was evaluated in terms of shape fidelity, applied extrusion pressure and post-printing cell viability. The line width and pore size of all the scaffolds were measured using Olympus IX71 microscope and cellSens Standard software (version 1.16; Tokyo, Japan). The printability (Pr) of Ink H4 and Ink H4-RGD were defined based on the square shape using the following mathematical function where A, C and L symbols indicate pore area, pore circularity and perimeter of the printed scaffold pore. Under ideal conditions, the printed lines of the constructs would be of square shape, and the Pr value was equal to 1. Larger Pr value indicates the greater gelation degree of the bioink and vice versa. For determining the Pr value of each print scaffold, perimeter and area of interconnected channels (n = 12), optical images of printed constructs were analyzed in Olympus IX71 microscope and cellSens Standard software (version 1.16; Tokyo, Japan). www.nature.com/scientificreports/ scaffold was covered with 500 µL organoid culture medium and then incubated at 37 °C and 5% CO 2 . Organoid cell culture medium was prepared from DMEM F-12/and RPMI with EGF (Epidermal growth factor), bFGF (basic fibroblast growth factor) and B-27 complement. The cell viability was evaluated before printing (simple gel cell mix) and after printing on day 1(immediately), 2, 4, 7 and 10 by using a live and dead cell assay kit. Briefly, printed cells were stained with 2 µM calcein-AM/4 µM EthD-III for 1 h and washed twice with serum free media. Thereafter, the images were acquired and analysed by using Olympus IX71 microscope and cellSens Standard software (version 1.16; Tokyo, Japan) respectively. Relative percentage of live and dead cells were determined by counting the cells using NIH ImageJ software (1.43u; https ://image j.nih.gov/ij). The shear thinning and recovery properties of the hydrogel were evaluated with repeated time-sweep and amplitude-sweep testing procedures at 25 °C and 37 °C. Briefly, the hydrogel sample was loaded on the bottom plate of the rheometer and tested under 0.1% shear strain for 10 min. First testing stage revealed the stability of the hydrogel and its ability to extrude easily. After first stage, an amplitude sweep was applied by increasing the shear strain from 0.1 to 500% within 4 min. This second stage mimicked the extrusion process, which makes hydrogel flow due to decrease in the elastic modulus when the shear strain was increased. Right after the amplitude sweep, the second time sweep test was immediately applied to evaluate the rapid recovery of the elastic modulus of the hydrogel after printing. The shear stress vs shear rate graph was represented on log-log plot and then the intercept and R 2 values were determined. The following adjustable parameters and terms; τ (shear stress), γ (shear rate), K (consistency index; gives an idea of the viscosity) and n (flow behaviour index; dimension less) were analysed by simple power law model i.e., τ = kγ n , where n < 1 denotes pseudoplastic and n > 1 indicates dilatants flow.

Rheological properties of Ink
To test the rheology of fully crosslinked hydrogel, about 1.2 mL hydrogel from either non crosslinked or partial crosslinked hydrogels (5:1 mix) was added to a 35 mm petri dish and then covered with 2 mL DMEM-F12 medium. The samples were incubated for 24 h and the rheology was evaluated with oscillation-time sweep procedure at 37 °C.
Stiffness and stability of printed cell laden scaffolds. The rheology of cell laden scaffolds was assessed using AR 1500Ex Rheometer (TA instrument, USA) with parallel-plate geometry (20 mm, taper angle of a = 0.0412 and rad = 2.36). Briefly, cells were printed with designed scaffolds of 20 mm diameter, 1 mm height and 45% infill density and were incubated in six well plates supplemented with DMEM-F12 organoid media at 37 °C and 5% CO 2 . Oscillation time sweep with a strain of 1% and angular frequency of 10 rad/s was used for cell laden stiffness evaluation and the stiffness was measured during day 1, 5, 10 and 15. Each cell laden scaffold was constructed from Ink H4-RGD with NSCLC-PDX cells (2 × 10 5 cells per scaffold). Characterisation of 3D spheroids by using NucBlue and actin green assay. Nucleus and Actin staining (NucBlue and Actin green assay) were performed to confirm the spheroids formation and their growth in the printed scaffolds. The media was removed from the scaffolds and then the scaffolds were subjected to fixation by using 4% formaldehyde for 1 h at room temperature and washed with 1 mL of HBSS (twice). The scaffolds were then permeabilized with 0.1% Triton X-100 and subsequently after washing with HBSS, staining with NucBlue and ActinGreen488 (Life Technologies) was performed according to the manufacturer's protocol. The assay was performed after 48 h, 72 h, on 5th day and 7th day. Images were then acquired by using Olympus IX71 microscope and cellSens Standard software (version 1.16; Tokyo, Japan).
Scanning electron microscopy (SEM) analysis of the spheroid structure. NSCLC-PDX spheroids (on the 10th day) were fixed with 4% glutaraldehyde for 30 min. Fixed spheroids were subsequently dehydrated with graded proportions of ethanol (25,50,75,95, and 100%). Afterwards, complete dried scaffolds were coated with palladium gold, and finally examined under a scanning electron microscope (JEOL) at an acceleration voltage of 5 kV.
Immunofluorescence staining of 3D spheroids for assessment of in vitro tumor microenvironment, which mimics the in vivo stromal characteristics. On the 7th day, printed cell-laden scaffolds (i.e., NSCLC PDX spheroids) were fixed with 4% formaldehyde for 30 min at 37 °C, washed thrice with PBST and permeabilized with 0.4% Triton for 30 min. The triton washed out and blocked with 5% BSA overnight, washed thrice with PBST and incubated with E-Cadherin-rabbit and Vimentin-rabbit overnight. Then the scaffolds were washed thrice with PBST and further stained with the secondary antibodies for 3 h. Finally, the scaffolds were washed thrice with PBST and stained with NucBlue for 30 min. Images were taken with Olympus IX71 microscope. www.nature.com/scientificreports/ Cytotoxicity assays. For cytotoxicity study, 4 mL of Ink H4-RGD was mixed uniformly with 800 µL cell suspension (containing 1.2 × 106 cells), loaded into the printing cartridge and then printed onto the 24 well plates with estimated cell density of 5 × 10 4 cells/scaffold. Each printed cell-laden scaffold was nourished with 250 µL of organoid medium every other day and incubated at 5% CO 2 and 37 °C. On day 5, the cell-laden scaffolds (with MDAMB-231 WT, NSCLC-PDX and HCC 827 cells) were treated with anticancer drugs erlotinib, DTX and DOX. DOX was not usually used against lung cancer and hence was not used for NSCLC-PDX). After 48 h incubation, the scaffolds were stained with 300 µL of MTT (0.05 mg/mL) for 4 h and the formazan crystals were dissolved with 250 µL of DMSO for 2 h. For comparison, conventional 2D cell culture models with equal cell density were also prepared for each cell line. Briefly, 5 × 10 4 cells were plated in 24 well plates and incubated at 37 °C and 5% CO 2 for 48 h. After 48 h, all the cells were treated with similar drugs (Erlotinib, DTX and DOX) separately. Then, MTT solution (0.05 mg/mL) was added for 3-4 h. Finally, the formazan crystals were dissolved with 250 µL of DMSO for 30 min. The absorbance was measured at a wavelength of 565 nm on a Fluoroskan Ascent FLTM instrument (Labsystem). Cytotoxic activity was expressed as the drug concentration that inhibited cell viability by 50% (IC 50 ).

Statistical analysis.
The experimental results were expressed as mean ± standard deviation. Statistical analyses between different groups were performed by one-way ANOVA. p value < 0.05 was considered as statistically significant.

Data availability
All the data generated or analyzed during this study are included in this published article (and its "Supplementary Information" files). www.nature.com/scientificreports/ Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons licence, and indicate if changes were made. The images or other third party material in this article are included in the article's Creative Commons licence, unless indicated otherwise in a credit line to the material. If material is not included in the article's Creative Commons licence and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this licence, visit http://creat iveco mmons .org/licen ses/by/4.0/.